5Hardening Temperatures The temperatures for hardening depend on the carbon content.Plain carbon steels below 0.4% will not harden by heat treatment.The temperature decreases from approx 820 deg C as carbon content increases from 0.4% up to 0.8%, where temperature is approx 780 deg C.Above 0.8% the temperature remains constant at 780 deg C.
6AusteniteThis is the structure of irons and steels at high temperatures (over 800 deg C).For quench hardening all the material must start as Austenite.Quenching causes the Austenite to be partially or totally transformed to Martensite.
7MartensiteOnly formed by very rapid cooling from the austenitic structure.Needs to be above the Critical Cooling Rate.
8The needle-like structure of martensite, the white areas are retained austenite.
9HardenabilityThis is dependent upon the chemical composition of the steel alloy.The addition of Nickel, Chromium and Molybdenum will slow the transformation to other phases and allow more martensite to form.Most heat treatable steels are alloys rather than plain carbon steels.
10Quenching Media Four commonly used quenching media: Brine – the fastest cooling rateWater – moderate cooling rateOil – slowest cooling rateGas – used in automatic furnaces, usually liquid nitrogen, can be very fast cooling. Too rapid cooling can cause cracking in complex and heavy sections.
11Depth of HardeningDue to the mass effect, not all the section of a large component may be hardened due to too slow a cooling rate.This may leave a soft core, or in extreme cases prevent hardening altogether.
12The Heat Treatment Process “Pearlite” (ductile)BCC + Fe3C with different microstructuresHow you heat treat makes all the difference to the steel you get“Martensite” (brittle)
13TemperingThe brittleness of martensite makes hardened steels unsuitable for most applications.This requires the steel to be tempered by re-heating to a lower temperature to reduce the hardness and improve the toughness. This treatment converts some of the martensite to another structure called bainite.
16NormalisingHeat to Upper Critical Temperature, at which point the structure is all AusteniteCool slowly in air.Structure will now be fine equi-axed pearlite.Used to restore the ductility of cold or hot worked materials whilst retaining other properties.
17AnnealingHeat to above Upper Critical Temperature, at which point the structure is all AusteniteCool very slowly in the furnace.Structure will now be large-grained pearlite.Used to improve the properties of cast and forged steels prior to machining.
18Grain GrowthA glass vial containing a liquid that foams. Shaking results in a fine foam, which slowly coarsens with time. The coarsening process is somewhat analogous to grain growth in solids.The same vial, after allowing some time for the foam to coarsen. The process occurs in order to reduce the surface per unit volume.
19SpheroidisingHeat to just below Lower Critical Temperature. (about deg C)Cool very slowly in the furnace.Structure will now be spheroidite, in which the Iron Carbide has ‘balled up’.Used to improve the properties of medium and high carbon steels prior to machining or cold working.
20Process (stress-relief) Annealing Heat to below Upper Critical Temperature to cause recrystallisationCool very slowly in the furnace.Structure will now be equi-axed pearlite.Used to maximise the ductility of low carbon steels and other materials after cold working.
21Cold Working Cold roll to “pancake” grains Increases hardness and strength at the expense of ductility.